Effects of Bonding Agents on Metal-Ceramic Bond Strength of Co-Cr Alloys Fabricated by Selective Laser Melting Soo-Yoen Yoo 1 , Seong-Kyun Kim 1, *, Seong-Joo Heo 1 , Jai-Young Koak 1 and Joung-Gyu Kim 2 1
Department of Prosthodontics and Dental Research Institute, Seoul National University Dental Hospital, School of Dentistry, Seoul National University, 101 Daehak-ro, Jongno-gu, Seoul 03080, Korea; [email protected]
(S.-Y.Y.); [email protected]
(S.-J.H.); [email protected]
(J.-Y.K.) Sense Dental Laboratory, 1104, Seoul Soop IT-Valley, 77, Seongsuil-ro, Seongdong-gu, Seoul 04790, Korea; [email protected]
Correspondence: [email protected]
; Tel.: +82-2-2072-3860
Received: 7 September 2020; Accepted: 24 September 2020; Published: 28 September 2020
Abstract: Bonding agents have been developed to improve bond strength between ceramic and Co-Cr metal. The aim of this study was to investigate the influence of two bonding agents on bond strength of Co-Cr metal fabricated by selective laser melting (SLM). Bond strength was determined by a three-point bending test, and the interfaces of the metal and ceramic, before and after the bending test, were observed by optical microscopy and scanning electron microscopy (SEM) to determine the thickness of the oxide layer and amount of ceramic remaining. To analyze the elemental composition of the bonding agents and fractured surfaces, energy dispersive X-ray spectroscopy (EDS) was used. Co-Cr specimens with bonding agent showed significantly higher bond strength than Co-Cr specimens without bonding agents. The fractured surfaces of most specimens showed mixed failure, but failure mode varied according to bonding agent and fabrication type. Specimens from groups treated with bonding agents had significantly higher remaining ceramic fractions on fractured Co-Cr alloys than specimens from groups that did not receive bonding agent. Mass amounts of silicone (Si) and titanium (Ti) on the fractured alloy surfaces were also different among specimens according to method of fabrication and presence of bonding agent. Together, the results suggest that application of bonding agent to 3D printed Co-Cr metal increases bond strength with ceramics. Keywords: cobalt-chromium (Co-Cr) alloy; selective laser melting (SLM); bond strength; metal bonding agent; three-point bending test; fracture failure mode
1. Introduction To reduce the risk of internal micro-cracking during the cooling phase of ceramic fabrication, porcelain-fused-to-metal (PFM) crowns were developed in the late 1950s. For 60 years, PFM has been the main type of prosthesis material used in dentistry, although recent studies have focused on development and improvement of metal-free esthetic restorations such as zirconia. However, base metal alloys are economical alternatives to gold alloys and zirconia. Furthermore, thinner and longer infrastructures can be fabricated using base metal alloys than zirconia and gold alloys because these base metal alloys have greater rigidity related to their modulus of elasticity . Ni-Cr alloy as a PFM framework was replaced by Co-Cr due to allergic and toxic reactions in the oral cavity. De Melo et al. investigated the bond strength of dental ceramic and demonstrated that it did not differ between Ni-Cr alloy and Co-Cr alloy . Heat-resistant and non-magnetic Co-Cr alloys have high strength and favorable resistance to wear, corrosion, and tarnish. Joias et al. found that the bond strength of ceramic to Co-Cr alloy depends on the alloy composition . Some studies have Materials 2020, 13, 4322; doi:10.3390/ma13194322
Materials 2020, 13, 4322
2 of 15
reported that the bond strength of ceramic to Co-Cr alloys fabricated using the lost wax technique ranges from 35 MPa to 95 MPa, which is an appropriate range for clinical applications [4–6]. The Co-Cr framework fabricated by casting is labor intensive and might amplify errors in the manufacturing process. Developments in dental technology over the past few decades have resulted in alternative restoration methods to the conventional lost wax technique for Co-Cr alloys. The first method involves computer-aided design—computer-aided manufacture (CAD-CAM) technology, while the other method is based on selective laser melting (SLM), commonly known as laser sintering. Both techniques are promising for further dental applications due to their cost and labor effectiveness. SLM restoration in particular is less expensive and time-consuming than the conventional lost wax technique without any compromise in quality of the final product. SLM also eliminates internal porosity and provides a single-phase microstructure, thereby preventing galvanic coupling within alloy phases . Co-Cr alloys fabricated by the SLM method exhibit better microstructures and mechanical properties than those fabricated by milling or casting . Although SLM appears to be a very promising technique, many other properties of the resulting materials, such as fit accuracy and metal-ceramic bond strength, need to be investigated in greater detail to validate SLM as a reliable alternative method to the conventional lost wax technique. The success of metal–ceramic prostheses depends primarily on optimal bond strength between the ceramic and metal components. The bonding behavior of ceramic to metal can be described both chemically and micro-mechanically. Oxide-forming constituents in the metal alloy form an appropriate thickness oxide layer on the metal surface. The veneering ceramic bonds to this oxide surface by a combination of mechanical retention, van der Waals interactions, and chemical bonding with the oxide layer, the latter making the most significant contribution to bond strength between ceramic and metal . Mechanical retention is another important determinant of bond strength. For stronger mechanical bonding, proper metal framework design, adequate veneering ceramic support, and adequate ceramic thickness are important . A higher surface roughness increases metal–ceramic bond strength due to improved mechanical interlocking between the metal and ceramic components. Therefore, sand blasting the metal alloy with airborne particles results in better bonding . A compatible coefficient of thermal expansion (CTE) between ceramic and metal is mandatory for successful PFM prostheses [11–13] as the CTE mismatches induce bonding failure. If the contraction of the alloy is greater than that of ceramic, during the cooling phase there will be compressive stress within the ceramic and tensile stress in the metal alloy. This compressive force on ceramic might close the primary flaws and crazing as well as prohibit crack propagation. Therefore, a slightly greater coefficient of thermal expansion of metal substrate than the ceramic is essential. The coefficient of thermal expansion may be influenced by inclusion of minor constituents such as aluminum (Al), Si, Ti within the composition of metal and ceramic. A typical range of the coefficient of thermal expansion for the porcelain is from 13.0 to 14.5 × 10−6 /◦ C, whereas that of the metal alloy typically has a slightly higher range of 13.5 to 14.9 × 10−6 /◦ C. Many studies on Co-Cr alloys fabricated by SLM have demonstrated that the bond strength of the ceramic to the SLM Co-Cr metal fulfills the ISO 9693-1 criterion for a minimum acceptable metal ceramic bond strength of 25 MPa. However, few studies have examined the bond strength of ceramic to SLM Co-Cr alloy after thermal aging to reproduce the actual oral environment, and clinicians and technicians often report bonding failure of ceramic to SLM Co-Cr alloys in practice [14–16]. Therefore, methods are needed to increase the bond strength of ceramic to Co-Cr alloy fabricated by SLM to withstand the stresses created in the dynamic environment of the oral cavity. McLean et al. reported that chromium oxide in Co-Cr adversely affected the bond strength by lowering the CTE of ceramic. In contrast, Cr might prevent formation of an excessive oxide layer, which weakens bond strength [17,18]. Isil et al. reported that silicone (Si) coating improved the bond strength and Wang et al. showed that Si3 N4 and Cr coating reduced the thickness of the oxide layer, resulting in stronger bonding [19,20]. Coating of chemical elements such as Au, Si, Ti on the metal substrate has also been shown to improve bond strength between ceramic and metal. Ceramic manufacturers have
Materials 2020, 13, x FOR PEER REVIEW Materials 2020, 13, 4322
3 of 16 3 of 15
substrate has also been shown to improve bond strength between ceramic and metal. Ceramic manufacturers haveseveral recently introduced several types bonding agents to improve bond recently introduced types of metal bonding agentsoftometal improve bond strength between ceramic strength between ceramic and metal. and metal. Our aiminin this study to evaluate the strength bond strength ofceramic dental to ceramic to Co-Cr alloy Our aim this study waswas to evaluate the bond of dental Co-Cr alloy fabricated fabricated by SLM after thermal aging of specimens to reproduce the oral environment. Additionally, by SLM after thermal aging of specimens to reproduce the oral environment. Additionally, we wanted weverify wanted verify that commercially available bonding agents SLMdid Co-Cr alloys increase to thattocommercially available bonding agents for SLM Co-Crfor alloys increase thedid strength of the strength of the bond between ceramic and SLM Co-Cr alloys as claimed by the manufacturers the bond between ceramic and SLM Co-Cr alloys as claimed by the manufacturers 2. Materials and Methods 2. A flow flow chart chart of of our our experimental experimental design designis is presented presentedin inFigure Figure1. 1. Co-Cr Co-Cr alloy alloy substrates substrates for for metal metal A bond strength strength tests tests were were fabricated fabricated by by two manufacturing methods (SLM and conventional casting). bond SLM-manufactured specimens specimens were divided divided into into three three groups groups based based on on application application of of our our bonding bonding SLM-manufactured agent and two commercial bonding agents. Groups and materials used in this study are shown in agent and two commercial bonding agents. study are shown in Table1.1. Table
Figure Figure 1. 1. Flow chart of the the bond bond strength strength experiments. experiments. Table 1. Specifications of the alloys, ceramic, and bonding agents used in this study. Table 1. Specifications of the alloys, ceramic, and bonding agents used in this study. Material
CTE (× 10−6 K−1 )
Material Material Type Brand Name Composition (wt%) CTE (× 10−6 K−1) Manufacturer Metal ingots: Co 59.4%, Cr 24.5%, W 10%, Nb2%, Dentsplysirona, Star Loy C 14.6~14.9 Metal ingots: Co 59.4%, Cr 24.5%, W 10%, Nb2%,V Dentsplysirona, casting V 2%, Other (Mo, Si, Fe) ≤ 1% Star Loy C 14.6~14.9 PA, USA Co-Cr alloy casting 2%,Other (Mo, Si, Fe) ≤ 1% PA, USA Scheftner dental alloys Metal powder: Starbond CoS Co 59%, Cr 25%, W 9.5%, Mo 3.5%, Co-Cr alloy 14.4 Scheftner dental Metal powder: Starbond CoS Co Si 59%, 25%, W 9.5%, Mo SLM powder 1%, Cr Other (C,Mn,Fe,N) ≤ 1%3.5%, Si 14.4 alloys SLM powder 1%, Other (C,Mn,Fe,N) ≤ 1% Vintage MP SiO Shofu, Dental GmbH 2 55–60%, Al2 O3 10–16%, Ceramic 13.6–15.2 Dental ceramic powder Shofu, K2 O 5–11%, Na2 O 2–16% Japan Dental Dental Vintage MP SiO2 55–60%, Al2O3 10–16%, Ceramic 13.6–15.2 GmbH Hersteller, Creation Willi ceramic powder proprietary 13.3 Metal bonding Meiningen, Austria Geller K 2O 5–11%, Na2O 2–16% Japan Bonding agent agent Hersteller, Davis Schottlander unmeasurable Matchmaker proprietary (≤14.4) 13.3 Letchworth, Herts, UK CTEWilli buffer Creation proprietary Meiningen, Austria Geller CTE: Coefficient of thermal expansion. Bonding Metal bonding agent agent Davis Schottlander Matchmaker CTE unmeasurable proprietary Letchworth, Herts, 2.1. Specimen Preparation andbuffer Analysis of Bonding Agents (≤14.4) UK
CTE: CoefficientBond of thermal expansion. 2.1.1. Specimen Preparation for Metal-Ceramic Strength Tests
In the present study, 20 metal substrates of Co-Cr alloy (Star Loy C, Dentsply Sirona, PA, USA) were fabricated using the lost wax technique, and 60 metal substrates of Co-Cr alloy (Starbond CoS powder, Scheftner Dental Alloys, Mainz, Germany) were fabricated using SLM (Concept Laser Mlab, Concept Laser GmbH, Lichtenfels, Germany). Substrates were fabricated to have a parallelepiped shape with a width of 3 mm, length of 25 mm, and thickness of 0.5 mm according to ISO 9693 specifications. The 60 SLM metal substrates were divided into three groups of 20 specimens each; one without bonding agent (only sandblasted) and one treated with each commercial bonding agent.
In the present study, 20 metal substrates of Co-Cr alloy (Star Loy C, Dentsply Sirona, PA, USA) were fabricated using the lost wax technique, and 60 metal substrates of Co-Cr alloy (Starbond CoS powder, Scheftner Dental Alloys, Mainz, Germany) were fabricated using SLM (Concept Laser Mlab, Concept Laser GmbH, Lichtenfels, Germany). Substrates were fabricated to have a parallelepiped shape with a width of 3 mm, length of 25 mm, and thickness of 0.5 mm according to ISO 9693 Materials 2020, 13, 4322 4 of 15 specifications. The 60 SLM metal substrates were divided into three groups of 20 specimens each; one without bonding agent (only sandblasted) and one treated with each commercial bonding agent. A single type of of dental porcelain with dimensions of 8of×83×× 31.1 mm waswas applied to the An A single type dental porcelain with dimensions × 1.1 mm applied to specimens. the specimens. illustration of aofspecimen used in the present study conforming to ISO 9693 guidelines is shown in An illustration a specimen used in the present study conforming to ISO 9693 guidelines is shown Figure 2. 2. Brand names, elemental in Figure Brand names, elementalcompositions compositionsofofthe thealloys, alloys,and andmanufacturers manufacturers are are provided in Table 1. 1. Table
Figure 2. Schematic diagram of metal-ceramic specimens conforming to ISO 9693 guidelines.
Figure 2. Schematic diagram of metal-ceramic specimens conforming to ISO 9693 guidelines.
Twenty wax models for metal alloy specimens were cast in a high-frequency electric heater (casting machine, Dental, Korea). There was no post-heat after cooling room Twenty wax Seki models for Seoul, metal alloy specimens were cast in a treatment high-frequency electricatheater temperature. SLM specimens were designed using CAD software (3shape CAD, 3shape, Copenhagen, (casting machine, Seki Dental, Seoul, Korea). There was no post-heat treatment after cooling at room Denmark), andSLM the data were transferred to a three-dimensional printing (3shape machine. CAD, Production of temperature. specimens were designed using CAD software 3shape, 60 samples of Denmark), 30 µm thickness wasdata carried outtransferred through melting and binding the Co-Cr-based metal Copenhagen, and the were to a three-dimensional printing machine. powder (Starbond CoS powder, Scheftner Dental Alloys, Mainz, Germany) in a selective laser sintering Production of 60 samples of 30 μm thickness was carried out through melting and binding the Codevice (Concept Mlab, ConceptCoS Laserpowder, GmbH, Lichtenfels, Germany) layerMainz, by layer in accordance Cr-based metal Laser powder (Starbond Scheftner Dental Alloys, Germany) in a with the virtual design. Parameters of the laser the firing schedule the metal frameworks selective laser sintering device (Concept Lasersystem Mlab,and Concept Laser GmbH,ofLichtenfels, Germany) were according to the manufacturer’s layer set-up by layer in accordance with the virtualrecommendations. design. Parameters of the laser system and the firing
schedule of the metal frameworks were set-up according to the manufacturer’s recommendations. 2.1.2. Analysis of Bonding Agent Surface 2.1.2.Two Analysis Bondingagents Agent Surface metalofbonding (shown in Table 1) were applied to specimens according to the manufacturers’ instructions. To determine which1)elements were present in the according bonding agents, Two metal bonding agents (shown in Table were applied to specimens to the we analyzed their surfaces using energy dispersive X-ray spectroscopy (EDS). manufacturers’ instructions. To determine which elements were present in the bonding agents, we analyzed their surfaces using energy dispersive X-ray spectroscopy (EDS). 2.1.3. Application of Veneering Ceramic ensure a flatofsurface without concavity or convexity, all metal specimens were inspected, and the 2.1.3.To Application Veneering Ceramic dimensions of samples were carefully measured with calipers (Dial Caliper, Starrett Company, Athol, To ensure a flat surface without concavity or convexity, all metal specimens were inspected, and MA, USA). Before the oxidation process, 80 Co-Cr metal samples were cleaned in an ultrasonic cleaner the dimensions of samples were carefully measured with calipers (Dial Caliper, Starrett Company, (BioSonic UC50, Coltène/Whaledent GmbH&Co. KG, Langenau, Germany) with distilled water for MA, USA). Before the oxidation process, 80 Co-Cr metal samples were cleaned in an ultrasonic 10 min, followed by washing with ethyl alcohol for 10 min to remove surface residue. After oxidation, cleaner (BioSonic UC50, Coltène/Whaledent GmbH&Co. KG, Langenau, Germany) with distilled samples were blasted with 50 µm Al2 O3 particles (Eazimill A11; Vericom, Korea) from a 1 cm distance water for 10 min, followed by washing with ethyl alcohol for 10 min to remove surface residue. After for 5 s under 4 atm pressure. The center 8 mm of the samples on one surface were measured for ceramic oxidation, samples were blasted with 50 μm Al2O3 particles (Eazimill A11; Vericom, Korea) from a application. Bonding agents A and B were applied to the 40 metal Co-Cr alloy plates produced by SLM before application of opaque porcelain according to the manufacturer’s instructions. Opaque porcelain was applied at the same place and with the same dimensions on 80 samples. Ceramic firing of the samples was performed in a ceramic furnace (Programat p500, Ivoclar Vivadent, Schaan, Liechtenstein) following the manufacturer’s instructions (shown in Table 2). Dimensions were measured with a micrometer (Dial Caliper, Starrett Company, Athol, MA, USA) to ensure that all fired samples had dimensions of 8 × 3 × 1.1 mm.
Dimensions were measured with a micrometer (Dial Caliper, Starrett Company, MA, USA) to ensure that all fired samples had dimensions of 8 × 3 × 1.1 mm. Table 2. Firing schedules for the veneering ceramic. Materials 2020, 13, 4322 Pre-Heating Temperature Drying Time Heating Rate Final Temperature (°C) (min) (°C/min) (°C) Liner (primer) 500 5 55 980 Table ceramic. 960 First opaque 500 2. Firing schedules 5 for the veneering 55 Second opaque 500 5 55 940 Pre-Heating Drying Time Heating55 Rate Final Temperature Dentin 500 5 920 ◦ (min) 5 (◦ C/min) (◦900 C) Glaze (self-glaze) Temperature 500( C) 55
5 of 15 Holding Time (min) 1 1 1 Holding 1 Time (min) 1
Liner (primer) 500 5 55 980 1 FirstTo opaque 500 5 960 ceramic bonding 1 surface determine the thickness of the oxide layer, we 55 examined the metal Second opaque 500 5 55 940 by field emission scanning electron microscopy (SEM) (ThermoFisher Scientific, Apreo S, 1MA, USA) Dentin 500 5 55 920 1 laterally after specimen500 surfaces were sputtered with an Glaze (self-glaze) 5 55 Au-layer (Polaron 900 SC 7620 Sputter 1 Coater,
Quorum Technologies Ltd., Kent, GB, UK) due to the low conductivity of porcelain. determine thickness of the oxideoflayer, we examined metalInterface ceramic bonding surface 2.2.To Bond Strengththe Test and Characterization the Co-Cr Metal andthe Ceramic by field emission scanning electron microscopy (SEM) (ThermoFisher Scientific, Apreo S, MA, USA) laterally after specimenBond surfaces were Test sputtered with an Au-layer (Polaron SC 7620 Sputter Coater, 2.2.1. Metal–Ceramic Strength Quorum Technologies Ltd., Kent, GB, UK) due to the low conductivity of porcelain. The three-point bending test performed according to the ISO 9693 standard is widely used to measure metal–ceramic bond strength (shown in Figure specimens were tested in 2.2. Bond Strength Test and Characterization of the Co-Cr Metal3). andCeramic Ceramicmetal Interface a desktop universal testing device (TW-D102, Taewon Tech, Seoul, Korea) with a head displacement 2.2.1. Metal–Ceramic Bond Strength Test speed of 1.0 mm/min. Samples with ceramic superstructures were placed face down on the device, which adjustedbending to a 20 mm between the two Thestandard load was is adjusted proceed The was three-point testdistance performed according to supports. the ISO 9693 widelyto used to at the rate of 1 mm/min vertically to the center of the metal surface on the specimens until breaking measure metal–ceramic bond strength (shown in Figure 3). Ceramic metal specimens were tested in a of the metal-ceramic interface The force (N) that caused crack initiation fracture on the metaldesktop universal testing devicebond. (TW-D102, Taewon Tech, Seoul, Korea) withor a head displacement ceramic interface was recorded byceramic software (Trapezium Xwere Material Testing Operation speed of 1.0 mm/min. Samples with superstructures placed face down on the Software, device, Shimadzu, Kyoto, Japan) on a computer connected to the universal testing device. which was adjusted to a 20 mm distance between the two supports. The load was adjusted to proceed 2) = k × F, Metal–ceramic bond strength (σ(MPa)) all specimens wasoncalculated as σ (N/mm at the rate of 1 mm/min vertically to the center of of the metal surface the specimens until breaking k is a constant related bond. to thickness and the of elasticity of the Co-Cr alloy, on andthe F is of where the metal-ceramic interface The force (N) modulus that caused crack initiation or fracture the load (in N) that causes de-bonding between metal and porcelain. In this study, the E-moduli metal-ceramic interface was recorded by software (Trapezium X Material Testing Operation Software,of Co-Cr specimens fabricated by conventional casting and SLM were 200 and 197.5 GPa, respectively. Shimadzu, Kyoto, Japan) on a computer connected to the universal testing device.
Figure 3. 3. Schematic diagram of of thethe three-point bending test. Figure Schematic diagram three-point bending test. 2 ) = k × F, Metal–ceramic bond strength (σ(MPa)) oftest, all specimens was calculated as σ (N/mm Before the metal–ceramic bond strength thermal cycling was performed to simulate the oral where k is a constant to thickness andstored the modulus of elasticity alloy, andaging F is the environment . related All specimens were in distilled water ofatthe 37Co-Cr °C. Thermal was load (in N) that causes de-bonding between metal and porcelain. In this study, the E-moduli of Co-Cr specimens fabricated by conventional casting and SLM were 200 and 197.5 GPa, respectively. Before the metal–ceramic bond strength test, thermal cycling was performed to simulate the oral environment . All specimens were stored in distilled water at 37 ◦ C. Thermal aging was performed by thermo-cycling using a thermo-cycling machine (Taewon Tech, Seoul, Korea) for 5000 cycles between 5◦ and 55 ◦ C (dwell time of 30 s). This procedure corresponds to a five-year period of oral temperature conditions . To avoid sample confusion during thermal cycling, samples from each of the four groups were placed in individual mesh bags.
Materials 2020, 13, 4322
6 of 15
2.2.2. Characterization of the Metal–Ceramic Interface After the three-point bending test, crack propagation between metal and ceramic was analyzed by SEM (magnification 1000×, 200×). Subsequently, the metal-ceramic surface was manually de-bonded and the fractured surface was examined using SEM (magnification 300×) and then analyzed with energy dispersive X-ray spectroscopy (EDS) to detect the elemental distribution on the fractured surface. An optical microscope (Olympus SZX10, Japan, magnification 8×) and software (Image J, NIH, MD, USA) were used to analyze the failure mode and area fraction of adherent ceramic after de-bonding. Three types of failure mode were considered: adhesive, where less than 20% of the bonding area was covered by remaining ceramic in the Co-Cr substrate surface; mixed, where more than 20% but less than 80% ceramic was present; and cohesive, where more than 80% of the alloy surface was covered by remaining ceramic . 2.3. Statistical Analysis Statistical tests were performed using SPSS (IBM SPSS statistics 22, IBM, NY, US) software for Windows. The Levene test was applied to assess the equality of variances, while bond strength data and the Si ratio of fractured surfaces were analyzed in independent groups using one-way analysis (ANOVA). Probability values of p < 0.05 were considered to be statistically significant. Multiple comparisons were made by Tukey’s adjustment test. 3. Results 3.1. Analysis of Bonding Agent Surface Table 3 shows the EDS results for the bonding agents used in this study. The two bonding agents had similar element compositions but different mass percentages of the elements. Bonding agent B had much more titanium (Ti) than bonding agent A (Table 3), whereas bonding agent A had more Si than bonding agent B. Table 3. Compositions and masses of the bonding agents used in this study. Mass Norm (%)
Bonding agent A Bonding agent B
3.2. Metal–Ceramic Bond Strength and Characterization of the Metal–Ceramic Interface 3.2.1. Metal–Ceramic Bond Strength The mean bond strengths of the cast and SLM specimens without bonding agent were 32.21 ± 6.88 MPa and 35.29 ± 6.57 MPa, respectively. SLM Co-Cr specimens to which bonding agent was applied had higher bond strength values of 38.38 ± 8.11 MPa (bonding agent A) and 42.56 ± 5.21 MPa (bonding agent B). All samples with bonding agents had significantly higher bond strength than samples without bonding agent. There was no difference in bond strength according to fabrication method. All specimens with bonding agent had a much higher bond strength than the 25 MPa required by ISO 9693. Bond strengths in the various specimen groups are summarized in Table 4.
Materials 2020, 13, x FOR PEER REVIEW Materials 2020, 13, 4322
7 of 16 7 of 15
Table 4. Metal–ceramic bond strength (mean ± standard deviation) and passing rate (≥25 MPa). Table 4. Metal–ceramic bond strength (mean ± standard deviation) and passing rate (≥25 MPa). Groups Groups Casting Casting SLM-fabricated SLM-fabricated without bonding agent withoutSLM-fabricated bonding agent with bonding agent A SLM-fabricated SLM-fabricated with bonding agent A with bonding SLM-fabricatedagent B
Bond Strength Bond(Mpa) Strength (Mpa)
Passing Rate ≥ 25 Mpa Passing Rate ≥ 25(%) Mpa (%)
32.21 ± 6.88 a 32.21 ± 6.88 a
35.29 ± 6.57 a 35.29 ± 6.57 a 38.38 ± 8.11 b
75 75 100
38.38 ± 8.11 b 42.56 ± 5.21 b
42.56 ± 5.21 b
p-Value p-Value vs. SLM-fabricated with bonding agent A: 0.002 vs. SLM-fabricated with bonding A: 0.002 vs. SLM-fabricated with bonding agent agent B < 0.001 vs. SLM-fabricated with bonding agent B < 0.001 vs. SLM-fabricated with bonding agent A: 0.027 SLM-fabricated bonding A: 0.027 vs. vs. SLM-fabricated withwith bonding agentagent B: 0.001 SLM-fabricated vs. vs. Casting group: 0.002with bonding agent B: 0.001 vs. vs. SLM-fabricated without Casting group: 0.002bonding agent: 0.027 vs. vs. Casting group < 0.001 SLM-fabricated without bonding agent: 0.027 vs. vs. SLM-fabricated without bonding agent: 0.001 Casting group < 0.001
with bonding agent Blowercase letters (a,b in the table) indicate vs.significant SLM-fabricated without(pbonding Different differences < 0.05).agent: 0.001 Different lowercase letters (a,b in the table) indicate significant differences (p < 0.05).
3.2.2. Metal–Ceramic Interface Examination 3.2.2.Figure Metal–Ceramic Interface Examination 4 shows cross sections of the metal–ceramic specimens before the three-point bending test. In specimens manufactured or SLM thatspecimens did not receive agent, abending thick oxide Figure 4 shows cross sectionsbyofcasting the metal–ceramic beforebonding the three-point test. layer was present between the ceramic and metal; however, specimens fabricated by SLM that In specimens manufactured by casting or SLM that did not receive bonding agent, a thick oxide layer received either bonding A and or Bmetal; had intimate connections the and received ceramic was present between theagent ceramic however, specimens between fabricated bymetal SLM that components either bonding agent A or B had intimate connections between the metal and ceramic components.
Figure Figure 4. 4. Scanning Scanning electron electron microscopy microscopy images images of of the the Co-Cr Co-Cr and and ceramic ceramic interface interface after after sputtering sputtering with with Au Au due due to the low conductivity of ceramic. (a) (a) Casted specimen, magnification 200×; 200×; (b) (b) casted casted specimen, specimen, magnification magnification 1000×; 1000×;(c) (c)SLM-fabricated SLM-fabricatedspecimen specimenwithout withoutbonding bonding agents, agents, magnification magnification 200×;(d) (d)SLM-fabricated SLM-fabricatedspecimen specimenwithout without bonding bonding agents, agents, magnification magnification 1000×; 1000×;(e) (e) SLM-fabricated SLM-fabricated 200×; specimen with with bonding bonding agent agent A, A, magnification magnification 200×; 200×;(f) (f)SLM-fabricated SLM-fabricatedspecimen specimenwith withbonding bondingagent agent specimen A, magnification magnification 1000×; 1000×;(g) (g) SLM-fabricated SLM-fabricatedspecimen specimenwith with bonding bonding agent agent B, B, magnification magnification 200×; 200×;(h) (h) A, SLM-fabricated specimen with bonding agent B, 1000×. The red arrows indicate the thick oxide layer SLM-fabricated specimen with bonding agent 1000×. The red arrows indicate the thick oxide layer that looks looks like like aa gap gap between between ceramic ceramic and and metal. metal. that
Cross-sectional images images of of the the metal–ceramic metal–ceramic specimens specimens after after the the three-point three-point bending bending test test are are Cross-sectional presented in inFigure Figure5. 5. specimens without bonding a large was presented ForFor castcast and and SLMSLM specimens without bonding agents,agents, a large gap was gap present, present, and cracks propagated smoothly along the metal-ceramic interface without adherent ceramic and cracks propagated smoothly along the metal-ceramic interface without adherent ceramic (Figure (FigureIn5a–d). In contrast, SLM specimens with bonding or B, cracks roughly with 5a–d). contrast, for SLMfor specimens with bonding agent Aagent or B,Acracks spreadspread roughly with some some remaining opaque ceramic and absence of cracks in some portions of the interface (Figure 5e–h). remaining opaque ceramic and absence of cracks in some portions of the interface (Figure 5e–h).
Materials Materials 2020, 2020, 13, 13, 4322 x FOR PEER REVIEW Materials 2020, 13, x FOR PEER REVIEW
88 of of 15 16 8 of 16
Figure 5. SEM images of specimens after the three-point bending test and before manual detachment Figure Figure 5. 5. SEM SEM images images of of specimens specimens after after the the three-point three-point bending bending test test and and before before manual manual detachment detachment of the ceramic portion. (a) Casted specimen, magnification 200×; (b) casted specimen, magnification of of the ceramic portion. (a) (a) Casted specimen, magnification 200×; 200×; (b) (b) casted casted specimen, specimen, magnification magnification 1000×; (c) selective laser melting (SLM)-fabricated specimen without bonding agents, magnification 1000×; 1000×; (c) (c) selective selective laser laser melting melting (SLM)-fabricated (SLM)-fabricated specimen specimen without without bonding bonding agents, agents, magnification magnification 200×; (d) SLM-fabricated specimen without bonding agents, magnification 1000×; (e) SLM-fabricated 200×;(d) (d)SLM-fabricated SLM-fabricated specimen specimen without without bonding bonding agents, agents, magnification 1000×; 1000×; (e) (e) SLM-fabricated SLM-fabricated 200×; specimen with bonding agent A, magnification 200×; (f) SLM-fabricated specimen with bonding agent specimenwith withbonding bondingagent agent magnification 200×; (f) SLM-fabricated specimen with bonding specimen A,A, magnification 200×; (f) SLM-fabricated specimen with bonding agent A, magnification 1000×; (g) SLM-fabricated specimen with bonding agent B, magnification 200×; (h) agent A, magnification (g) SLM-fabricated specimen bonding B, magnification 200×; A, magnification 1000×;1000×; (g) SLM-fabricated specimen with with bonding agentagent B, magnification 200×; (h) SLM-fabricated specimen with bonding agent B, magnification 1000×. Dotted lines represent the (h) SLM-fabricated specimen with bonding agent magnification1000×. 1000×.Dotted Dottedlines linesrepresent represent the the SLM-fabricated specimen with bonding agent B,B,magnification surface of the Co-Cr alloy. Yellow triangles indicate crack propagation and the large gap between the surface of of the the Co-Cr Co-Cr alloy. alloy. Yellow Yellow triangles indicate crack propagation and the large large gap gap between between the the surface ceramic and metal layers. Red triangles indicate incomplete crack propagation. ceramic and metal layers. Red Red triangles triangles indicate indicate incomplete incomplete crack crack propagation. propagation. ceramic
3.2.3. Observation of the Fractured Surface 3.2.3. Observation of the Fractured Surface Figure 6 shows the Co-Cr substrate surfaces of specimens after de-bonding from the ceramic. ceramic. Figure 6 shows the Co-Cr substrate surfaces of specimens after de-bonding from the ceramic. After the the three-point three-point bending bending test, test, cracked cracked specimens specimens were manually manually de-bonded de-bonded to analyze analyze the the After After the three-point bending test, cracked specimens were manually de-bonded to analyze the the metal metal surface. surface. Visual inspection and optical microscopy remaining ceramic area proportions on the remaining ceramic area proportions on the metal surface. Visual inspection and optical microscopy were used usedto toobserve observethe thefractured fracturedsurfaces. surfaces.There Therewas wasmore moreadherent adherent ceramic alloy surface were ceramic onon thethe alloy surface in were used to observe the fractured surfaces. There was more adherent ceramic on the alloy surface in the SLM groups with different bonding agents than other groups. the SLM groups with different bonding agents than thethe other groups. in the SLM groups with different bonding agents than the other groups.
Figure 6. Optical microphotographs microphotographs of of Co-Cr Co-Cr alloy alloy surfaces surfaces after de-bonding with ceramic 6. Optical ceramic Figure 6. Optical microphotographs of Co-Cr alloy surfaces after de-bonding with ceramic (magnification 8×). (a)(a)Casted Castedspecimen; specimen;(b)(b) SLM-fabricated specimen without bonding agent; (magnification 8×). SLM-fabricated specimen without bonding agent; (c) (magnification 8×). (a) Casted specimen; (b) SLM-fabricated specimen without bonding agent; (c) (c) SLM-fabricated specimen with bonding agent A; (d) SLM-fabricated specimen with bonding agent SLM-fabricated specimen with bonding agent A; (d) SLM-fabricated specimen with bonding agent B. SLM-fabricated specimen with bonding agent A; (d) SLM-fabricated specimen with bonding agent B. B. Yellow triangles representadherent adherentceramic, ceramic,and andred redasterisks asterisks indicate indicate remnant remnant wash opaque. Yellow triangles represent opaque. Blue Yellow triangles represent adherent ceramic, and red asterisks indicate remnant wash opaque. Blue circles circles indicate indicate remnant remnant sputtered sputtered Au. Au. circles indicate remnant sputtered Au.
Failure Failure mode mode was was classified classified as as cohesive cohesive (fracture (fracture inside inside ceramic ceramic layers), layers), adhesive adhesive (fracture (fracture Failure mode ceramic was classified as cohesive (fracture inside ceramic layers), adhesive (fracture interface between and metal), or mixed (cohesive and adhesive failure) by analyzing interface between ceramic and metal), or mixed (cohesive and adhesive failure) by analyzing the the interface between ceramic andwith metal), or mixed adhesive failure) by analyzing the ceramic The SLM SLM bonding agent(cohesive B group group and showed no ceramic remnants. remnants. The with bonding agent B showed no adhesive adhesive failure failure and and some some ceramic remnants. The SLM with bonding agent B group showed no adhesive failure and some cohesive failure. Fracture modes are presented in Table 5. The mean amount of ceramic remaining cohesive failure. Fracture modes are presented in Table 5. The mean amount of ceramic remaining
Materials 2020, 13, 4322
9 of 15
Materials 2020, 13, x FOR PEER REVIEW
9 of 16
cohesive failure. Fracture modes are presented in Table 5. The mean amount of ceramic remaining was was significantly larger in groups bonding agents than in those without. Furthermore, significantly larger in groups with with bonding agents than in those without. Furthermore, there there were were significant differences in fracture modes between the two commercial bonding agents. significant differences in fracture modes between the two commercial bonding agents. Table Table 5. 5. Results Results of of failure failure mode mode analysis. analysis. Groups MixedFailure Failure Groups Mixed Casting 2 Casting 2 SLM-fabricated 8 SLM-fabricated without bonding agent 8 without bonding agent SLM-fabricated SLM-fabricated 1616 bonding agent withwith bonding agent A A SLM-fabricated SLM-fabricated 1414 bonding agent withwith bonding agent B B
CohesiveFailure Failure Adhesive Ceramic Fraction (%) (%) Cohesive AdhesiveFailureMean Failure Mean Ceramic Fraction 1 17 19.6 ± 17.12 a 1 17 19.6 ± 17.12 a 0 12 20.4 ± 10.22 a 0 12 20.4 ± 10.22 a
40.5 ±40.5 18.77 b ± 18.77 b
59.6559.65 ± 21.24 c ± 21.24 c
Different lowercase letters (a,b,c significantly different groups (p < 0.05). Different lowercase letters (a,b,cinintable) table) indicate indicate significantly different groups (p < 0.05).
SEM SEM images images (magnification (magnification 300×) 300×)of ofremnant remnantceramic ceramicon onthe theCo-Cr Co-Crmetal metalare areshown shownin inFigure Figure7.7. White areas represent adherent opaque and dentine ceramic on the alloy (light due to the low White areas represent adherent opaque and dentine ceramic on the alloy (light due to the low electrical electrical conductivity of the ceramic), while gray areas indicate Co-Cr alloy (dark due to the high conductivity of the ceramic), while gray areas indicate Co-Cr alloy (dark due to the high electrical electrical conductivity of the alloy). SLM-fabricated specimens with bonding agent B more showed more conductivity of the alloy). SLM-fabricated specimens with bonding agent B showed remnant remnant ceramic than the other groups ceramic than the other groups.
Figure 7. Scanning electron microscopy images (300×) of specimens after de-bonding of ceramic from Figure 7. Scanning electron microscopy images (300×) of specimens after de-bonding of ceramic from the Co-Cr alloy surface. (a) Casting group; (b) SLM-fabricated specimens without bonding agent; the Co-Cr alloy surface. (a) Casting group; (b) SLM-fabricated specimens without bonding agent; (c) (c) SLM-fabricated specimens with bonding agent A; (d) SLM-fabricated specimens with bonding SLM-fabricated specimens with bonding agent A; (d) SLM-fabricated specimens with bonding agent agent B. Red asterisks represent adherent ceramic. Yellow triangles show Co-Cr substrate fabricated B. Red asterisks represent adherent ceramic. Yellow triangles show Co-Cr substrate fabricated by by casting, and yellow circles indicate Co-Cr alloy fabricated by SLM. Blue diamonds indicate wash casting, and yellow Co-Cr alloy by SLM. Blue diamonds indicate wash opaque from ceramiccircles on the indicate Co-Cr substrate, whilefabricated green arrows indicate remnant Au from sputtering. opaque from ceramic on the Co-Cr substrate, while green arrows indicate remnant Au from sputtering. EDS analysis results for the fractured surfaces are presented in Figure 8 and Table 6. Based on
amount of Si present in representative SEM micrographs, the SLM group with bonding agent B had analysis results forthe theother fractured surfaces are presented in Figure 8 and Table 6. Based on moreEDS adherent ceramic than groups. amount of Si present in representative SEM micrographs, the SLM group with bonding agent B had more adherent ceramic than the other groups.
Materials 2020, 13, 4322 Materials 2020, 13, x FOR PEER REVIEW
10 of 15 10 of 16
Figure the fractured fractured Co-Cr Co-Cr and andceramic ceramicinterface. interface.(a)(a) Casted group specimens; Figure8.8.EDS EDS analysis analysis of of the Casted group specimens; (b) (b) SLM-fabricated specimens without bonding agent; (c) SLM-fabricated specimens bonding SLM-fabricated specimens without bonding agent; (c) SLM-fabricated specimens withwith bonding agent agent (d) SLM-fabricated specimens bonding A; (d)A;SLM-fabricated specimens with with bonding agentagent B. B. Table 6. EDS analysis results for the fracture surfaces (mean ± standard deviation). Table 6. EDS analysis results for the fracture surfaces (mean ± standard deviation). Specimen Groups O Al Si Zr Ti
Casting 43.18 ± 1.00 7.53 ± 1.00 18.91 ± 0.84 5.23 ± 2.19 2.34 ± 4.84 Casting 43.18 ± 1.00 7.53 ± 1.00 18.91 ± 0.84 5.23 ± 2.19 2.34 ± 4.84 SLM-fabricated 37.69 ± 7.58 7.65 ± 1.13 16.37 ± 1.94 2.2 ± 3.01 3.04 ± 1.20 SLM-fabricated without bonding agent 37.69 ± 7.58 7.65 ± 1.13 16.37 ± 1.94 2.2 ± 3.01 3.04 ± 1.20 without bonding agent SLM-fabricated 53.32 ± 5.73 7.02 ± 1.61 17.21 ± 2.73 3.29 ± 0.56 2.53 ± 4.39 with bonding agent A SLM-fabricated 53.32 ± 5.73 7.02 ± 1.61 17.21 ± 2.73 3.29 ± 0.56 2.53 ± 4.39 SLM-fabricated with bonding agent A ± 0.17 49.18 7.99 ± 2.33 22.56 ± 2.54 3.21 ± 1.44 5.8 ± 1.73 with bonding agent B
SLM-fabricated 49.18 ± 0.17 7.99 ± 2.33 22.56 ± 2.54 3.21 ± 1.44 5.8 ± 1.73 with bonding agent B 4. Discussion
4. Discussion Bond strength is determined by various factors including mechanical and micromechanical retention, der Waals interactionsby andvarious chemical bonding in the oxide layer, and CTE Bondvan strength is determined factors including mechanical and appropriate micromechanical differences between ceramic and metal components [8–11]. To evaluate the bond strength between retention, van der Waals interactions and chemical bonding in the oxide layer, and appropriate CTE ceramic and metal, weceramic fabricated by the[8–11]. conventional lost wax method,between which differences between andCo-Cr metalsamples components To evaluate the casting bond strength has been verified to be suitable for fabrication of specimens for use in a clinical setting, and the SLM ceramic and metal, we fabricated Co-Cr samples by the conventional lost wax casting method, which method, newer fabrication method. All metal specimens in our study sandblasted withthe 50 SLM um has beena verified to be suitable for fabrication of specimens for use in were a clinical setting, and Al O particles for 5 s to control surface roughness. Previous studies reported that airborne-particle 2 3 method, a newer fabrication method. All metal specimens in our study were sandblasted with 50 um abrasion with 50 particles shear bond strength ofthat porcelain to Co-Cr Al2O3 particles forµm 5 salumina to control surface improved roughness.the Previous studies reported airborne-particle alloy [24–26] by50 increasing the surface theshear metal, facilitating retention abrasion with μm alumina particlesroughness improvedofthe bond strengthmicromechanical of porcelain to Co-Cr alloy of[24–26] the porcelain and enhancing the wettability of porcelain on metal [25,27]. Opaque porcelain by increasing the surface roughness of the metal, facilitating micromechanical retentionflows of the into the microgrooves created sandblasting on the surface of the alloy Opaque and mechanically porcelain and enhancing theby wettability of porcelain on metal [25,27]. porcelaininterlocks flows into into the undercuts . All specimens in this study were abraded with airborne particles, avoiding the microgrooves created by sandblasting on the surface of the alloy and mechanically interlocks into differences in mechanical among SLM fabrication groups (the this is theavoiding casted the undercuts . All retention specimens in this study were abraded withexception airbornetoparticles, group, whichinhad differentretention metal properties). In our study, the main(the determinants ofthis bond strength differences mechanical among SLM fabrication groups exception to is the casted group, which had different metal properties). In our study, the main determinants of bond strength
Materials 2020, 13, 4322
11 of 15
were compressive bonding due to differences in CTE between metal and ceramic and chemical bonding within the oxide layer. Differences in CTE values induce stress and principally affect the interfacial bond strength that causes ceramic de-lamination or cracking, emphasizing the importance of a compatible CTE between veneering porcelain and Co-Cr alloy. It is essential that the metal substrate has a slightly greater CTE than the ceramic. The CTE can be influenced by minor constituents present in the metal and ceramic. The bonding agents we used in this study were developed to compensate for differences in CTE value between ceramic and metal. Our finding that the specimens to which these bonding agents were applied had higher bond strengths than specimens that did not receive application of these bonding agents indicates that the bonding agents increased bond strength. Deviations in in vitro and in vivo performances of restorations can result in differences in reported metal–ceramic bond strengths . It is impossible to simulate intraoral conditions perfectly due to all the factors necessary for fatigue-related failures in dental prostheses. In this in vitro study, we attempted to simulate the complexity of the oral environment in terms of temperature and moisture. Therefore, all specimens in this study were subjected to thermal cycling, which can potentially weaken metal–ceramic bonding [24,29,30]. The thermal aging procedure we used was based on previous studies; in particular, the lowest temperature for thermal cycle tests should be 5 ◦ C and the highest 55 ◦ C, with an average retention time of 30 s [24,31–33]. All samples in this study underwent 5000 cycles of exposure to 5 ◦ C and 55 ◦ C in accordance with ISO/TS 11,405 recommendations. Thermal cycling tests induce repeated stresses at the interface of two materials. Such stresses arise due to differences in thermal expansion coefficients of the two materials and can lead to adhesion losses . We examined bond strength by three-point bending testing using a universal testing machine. Despite lack of an ideal testing method , we used the three-point bending test in this study to determine metal-to-porcelain bond strength because metal and ceramic bond strength tests should be quantifiable, reproducible, and easy to perform ; in addition, this test is recommended by the American Dental Association Council on Dental Materials, Instruments, and Equipment. We found that ceramic and metal bond strengths differed slightly according to fabrication method but without statistical significance. In a similar study, Han et al. reported that bond strength values of samples produced with 3D printer were higher than those produced by the traditional casting method or CAD/CAM . A previous study also reported that SLM metal alloy showed better mechanical microstructure and properties than cast alloy , consistent with our findings that the bond strength of specimens fabricated using SLM alloy were slightly higher than those made by casting Co-Cr alloy. Notably, all Co-Cr substrates with bonding agent showed significantly higher bond strength than substrates without bonding agent. This supports the suggestion of the manufacturers that metal bonding agents affect bond strength by reducing the thickness of the oxide layer and compensating for differences in coefficient of temperature expansion between ceramic and Co-Cr alloy. A previous study reported that use of a metal bonding agent increased the Weibull modulus . This means that the presence of bonding agent narrowed the scatter of values of bond strength; in other words, a more reliable interface between ceramic and metal was produced. A related bond strength study reported a significantly higher bond strength between ceramic and Co-Cr alloy when a metal bonding agent was used . The present study differs from previous studies in that we subjected specimens to thermo-cycling to simulate the oral environment; nevertheless, all specimens with bonding agents had values that were remarkably higher than the minimum 25 MPa value required by ISO 9693 specifications. Some specimens without bonding agents showed inappropriate bond strength regardless of fabrication method. We investigated the fracture mode between ceramic and metal after the three-point bending test. Previous studies have reported that mixed type failure mode is the most frequent [25,34]. Conversely, another study found a mixed mode of failure in specimens fabricated with the casting technique, while specimens fabricated by the SLM technique had either mixed or adhesive mode of failure . Han et al. reported all adhesive failures in their study regardless of fabrication technique .
Materials 2020, 13, 4322
12 of 15
Under an optical microscope, most specimens with bonding agent B had an opaque layer and ceramic on the surface of the metal, suggesting mixed and cohesive failure mode, which was not seen in other groups. Specimens without bonding agents showed mostly adhesive failure mode, implying that cracks occurred between the metal and ceramic, and that there may have been some mixed failure modes . Adhesive failure is usually not an ideal situation because it indicates a lower bond strength between metal and ceramic than that within the ceramic interior; this requires less destructive force to separate metal and ceramic . In addition to the bond strength results reported here, fracture surface analysis results indicated that use of bonding agents increased the bond strength between ceramic and metal. EDS analysis showed that elements of porcelain, such as aluminum (Al), Si, and Ti, were present on the fractured Co-Cr alloy surfaces. The presence of Al might be due to remnants of the Al2 O3 air-particle abrasion process and/or porcelain (opaque layer) adhered to the alloy substrate. In our study, as Al compositions among groups were similar, we concluded that most of the Al was contributed by remnant Al2 O3 particles after air-particle abrasion. Si-containing metal bonding agents absorb excessive oxides that form on the alloy surface during porcelain firing [29,41]. As shown in Table 3, the bonding agents used in our study contained Si to improve bond strength by regulating the thickness of the oxide layer. The Si present on EDS after the stress test indicated remnant ceramic. The amount of Si on the fractured surfaces was greatest for SLM-fabricated alloy with bonding agent B (Figure 7 and Table 6), indicating that specimens in this group had the strongest bond strength in our study. We used Ti-containing bonding agents in this study (Table 3) as they act as oxygen scavengers to protect the alloy surface from progressive accumulation of an excessive oxidation layer with repetitive firing cycles [27,41,42]. A previous study suggested that titanium–ceramic adhesion involves a chemical reaction between Ti and Si, resulting in formation of a new Ti5 Si3 O phase . Chemical bonding with Ti is possible because of diffusion of porcelain components into titanium oxides during firing [44,45]. This phenomenon could be partially responsible for the increased metal–ceramic bond strength that we observed with bonding agent on the Co-Cr metal substrate. Different commercial bonding agents affect bond strength between ceramic and metal components differently; however, a bonding agent that contains Ti can moderate strong oxidation of the metal surface and increase bond strength. In other words, the bonding agent can function as a chemical bridge between ceramic and metal. Lu et al. linked the dynamic functional theory (DFT)-predicted adhesive energy at solid/liquid interface and cohesive energy at liquid/liquid interface with DFT atomic force microscope (AFM)-predicted force of adhesion through the Young–Dupré equation and established the basis of quantum surface wettability theory by combining two independent atomic-level quantum physics simulation methodologies . They used quantum physics via density functional theory simulation  to directly evaluate how the surface wettability of graphite is influenced. The wettability of ceramic to metal examined higher, where an active element, e.g., Al, Zr and Ti, alters the surface chemistry of the ceramic by the formation of intermediate reaction layer and lowers the wetting angle on the ceramic . In our study, SLM-fabricated with bonding agent group B showed highest values of Al and Ti (shown in Table 6). This physical property may also have effects on the positive increase of the bond strength between ceramic and Co-Cr alloy. Quantum chemical calculations at DFT level will help improve interpretation of the results in further research. Prior to performing three-point bending tests, we inspected the ceramic and metal bonding surfaces by SEM. As shown in Figure 3, for specimens produced by casting and SLM without bonding agent, there was a thick oxide layer which looked like a gap between the metal and ceramic in which ion-covalent bonds dominated. According to the manufacturers, bonding agents aim to close (or adequately reduce) this gap. This results in a corresponding increase in bond strength, consistent with our findings (Table 4). Even though differences in the main components of commercial bonding agents can result in differences in bond strength, we observed no significant differences between the two
Materials 2020, 13, 4322
13 of 15
commercial bonding agents in this study. Therefore, we recommend using either of these two bonding agents to increase bond strength. In this study, Concept Laser was used to print the Co-Cr alloy by SLM method with Star bond CoS powder and configured to build layers of 30 µm thickness. The study conducted by de Melo et al. found that rather than differences in layer thicknesses, variations in operating principles of devices used in production of metal and differences in the contents of alloy powders significantly affect metal-to-porcelain bonding . Therefore, different results would be observed if a different powder and/or printing device were used. Additionally, our study did not involve a fatigue procedure, therefore results remain optimistic to a certain extent, as physiochemical changes in dental materials attribute to a dynamic oral environment. Further study reproducing oral conditions based on thermal and mechanical cycling process should be considered. Regardless of the limitations of this study, we can apply bonding agents to increase the bond strength between ceramic and Co-Cr SLM alloy in the era of upcoming 3D printing. As we verified, the bond strength values for the groups with application of bonding agents were significantly higher than groups without it thanks to the oxide layer formation of appropriate thickness and compensation for differences in CTE value. Therefore, by using bonding agents, we assumed the long span prostheses which might contain more internal stress and the implant prostheses which do not have any capability to absorb excessive loading due to the lack of periodontal ligament can have more advantages. For greater bond strength between ceramic and Co-Cr alloy, the frequency of the chipping or delamination of ceramic would be remarkably reduced. 5. Conclusions We found that use of both commercial bonding agents significantly increased the bond strength between ceramic and SLM-produced metal alloys. All specimens from the groups in which bonding agents were used had a bond strength higher than 25 MPa, which is clinically acceptable. Although the fractured surfaces of specimens after three-point bending tests showed different characteristics depending on type of bonding agent used (there was no unfavorable adhesive failure for bonding agent group B; whereas, 20% of bonding agent group A showed adhesive failure), both commercial bonding agents we evaluated improved bond strength, indicating suitability of use of either bonding agent. This study does have its limitations, but we are able to determine that the use of bonding agent between ceramic and SLM would be helpful for clinicians to make long-term sustainable long-span prostheses of supporting strut that are fabricated by SLM. Author Contributions: Conceptualization, S.-Y.Y.; Methodology, S.-K.K. and J.-Y.K.; Software, S.-J.H. and J.-G.K.; Validation, S.-K.K. and J.-Y.K.; Formal Analysis, S.-Y.Y. and J.-G.K.; Investigation, S.-Y.Y. and J.-G.K.; Resources, S.-K.K. and, S.-J.H.; Data Curation, S.-Y.Y. and S.-J.H.; Writing—Original Draft Preparation, S.-Y.Y. and S.-K.K.; Writing—Review & Editing, S.-Y.Y. and J.-Y.K.; Visualization, S.-Y.Y. and S.-K.K.; Supervision, S.-K.K. All authors have read and agreed to the published version of the manuscript. Funding: This research was supported by the Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education (NRF-2018R1D1A1B07042333). Conflicts of Interest: The authors declare no conflict of interest.
References 1. 2. 3.
Al Jabbari, Y.S. Physico-mechanical properties and prosthodontic applications of Co-Cr dental alloys: A review of the literature. J. Adv. Prosthodont. 2014, 6, 138–145. [CrossRef] [PubMed] Melo, R.; Travassos, A.C.; Neisser, M.P. Shear bond strengths of a ceramic system to alternative metal alloys. J. Prosthet. Dent. 2005, 93, 64–69. [CrossRef] Joias, R.; Tango, R.; DeAraujo, J.; DeAraujo, M.; De Siqueira Ferreira Anzaloni Saavedra, G.; De Arruda Paes-Junior, T.; Kimpara, E. Shear bond strength of a ceramic to Co-Cr alloys. J. Prosthet. Dent. 2008, 99, 54–59. [CrossRef]
Materials 2020, 13, 4322
4. 5. 6.
7. 8. 9. 10. 11. 12. 13. 14. 15. 16.
17. 18. 19. 20. 21. 22. 23.
26. 27. 28.
14 of 15
Bezzon, O.L.; Ribeiro, R.F.; Rollo, J.M.D.D.A.; Crosara, S.; Crosarad, S. Castability and resistance of ceramometal bonding in Ni-Cr and Ni-Cr-Be alloys. J. Prosthet. Dent. 2001, 85, 299–304. [CrossRef] Lacy, A.M. The chemical nature of dental porcelain. Dent. Clin. N. Am. 1977, 21, 661–667. Hofstede, T.M.; Ercoli, C.; Graser, G.N.; Tallents, R.H.; Moss, M.E.; Zero, D.T. Influence of metal surface finishing on porcelain porosity and beam failure loads at the metal-ceramic interface. J. Prosthet. Dent. 2000, 84, 309–317. [CrossRef] Zhou, Y.; Li, N.; Yan, J.; Zeng, Q. Comparative analysis of the microstructures and mechanical properties of Co-Cr dental alloys fabricated by different methods. J. Prosthet. Dent. 2018, 120, 617–623. [CrossRef] McLean, J.W.; Hughes, T.H. The reinforcement of dental porcelain with ceramic oxides. Br. Dent. J. 1965, 119, 251–267. Sailer, I.; Fehér, A.; Filser, F.; Lüthy, H.; Gauckler, L.J.; Schärer, P.; Hämmerle, C.H.F. Prospective clinical study of zirconia posterior fixed partial dentures: 3-year follow-up. Quintessence Int. 2006, 37, 685–693. Uusalo, E.K.; Lassila, V.P.; Yli-Urpo, A.U. Bonding of dental porcelain to ceramic-metal alloys. J. Prosthet. Dent. 1987, 57, 26–29. [CrossRef] Knap, F.J.; Ryge, G. Study of Bond Strength of Dental Porcelain Fused to Metal. J. Dent. Res. 1966, 45, 1047–1051. [CrossRef] Hong, J.-M.; Razzoog, M.E.; Lang, B.R. The effect of recasting on the oxidation layer of a palladium-silver porcelain alloy. J. Prosthet. Dent. 1988, 59, 420–425. [CrossRef] McLean, J.W. Ceramics in clinical dentistry. Br. Dent. J. 1988, 164, 310. [CrossRef] [PubMed] Li, J.; Chen, C.; Liao, J.; Liu, L.; Ye, X.; Lin, S.; Ye, J.-T. Bond strengths of porcelain to cobalt-chromium alloys made by casting, milling, and selective laser melting. J. Prosthet. Dent. 2016, 118, 69–75. [CrossRef] [PubMed] Akova, T.; Ucar, Y.; Tukay, A.; Balkaya, M.C.; Brantley, W.A. Comparison of the bond strength of laser-sintered and cast base metal dental alloys to porcelain. Dent. Mater. 2008, 24, 1400–1404. [CrossRef] Wu, L.; Zhu, H.; Gai, X.; Wang, Y. Evaluation of the mechanical properties and porcelain bond strength of cobalt-chromium dental alloy fabricated by selective laser melting. J. Prosthet. Dent. 2014, 111, 51–55. [CrossRef] McLean, J.W. The metal-ceramic restoration. Dent. Clin. N. Am. 1983, 27, 747–761. Sced, I.R.; McLean, J.W. The strength of metal-ceramic bonds with base metals containing chromium. A preliminary report. Br. Dent. J. 1972, 132, 232–234. [CrossRef] Özcan, I.; Uysal, H. Effects of silicon coating on bond strength of two different titanium ceramic to titanium. Dent. Mater. 2005, 21, 773–779. [CrossRef] Wang, R.R.; Welsch, G.; Monteiro, O. Silicon nitride coating on titanium to enable titanium-ceramic bonding. J. Biomed. Mater. Res. 1999, 46, 262–270. [CrossRef] Gale, M.S.; Darvell, B.W. Thermal cycling procedures for laboratory testing of dental restorations. J. Dent. 1999, 27, 89–99. [CrossRef] Schneider, R.L.; Curtis, E.R.; Clancy, J.M. Tensile bond strength of acrylic resin denture teeth to a microwaveor heat-processed denture base. J. Prosthet. Dent. 2002, 88, 145–150. [CrossRef] [PubMed] Han, X.; Sawada, T.; Schille, C.; Schweizer, E.; Scheideler, L.; Geis-Gerstorfer, J.; Rupp, F.; Spintzyk, S. Comparative Analysis of Mechanical Properties and Metal-Ceramic Bond Strength of Co-Cr Dental Alloy Fabricated by Different Manufacturing Processes. Materials 2018, 11, 1801. [CrossRef] [PubMed] Vásquez, V.Z.C.; Özcan, M.; Kimpara, E.T. Evaluation of interface characterization and adhesion of glass ceramics to commercially pure titanium and gold alloy after thermal- and mechanical-loading. Dent. Mater. 2009, 25, 221–231. [CrossRef] Lombardo, G.H.L.; Nishioka, R.S.; Souza, R.O.D.A.E.; Michida, S.M.A.; Kojima, A.N.; Mesquita, A.M.M.; Buso, L. Influence of Surface Treatment on the Shear Bond Strength of Ceramics Fused to Cobalt-Chromium. J. Prosthodont. 2010, 19, 103–111. [CrossRef] Saito, A.; Komine, F.; Blatz, M.B.; Matsumura, H. A comparison of bond strength of layered veneering porcelains to zirconia and metal. J. Prosthet. Dent. 2010, 104, 247–257. [CrossRef] Al Hussaini, I.; Al Wazzan, K.A. Effect of surface treatment on bond strength of low-fusing porcelain to commercially pure titanium. J. Prosthet. Dent. 2005, 94, 350–356. [CrossRef] Vásquez, V.; Özcan, M.; Nishioka, R.; Souza, R.O.D.A.E.; Mesquita, A.; Pavanelli, C. Mechanical and thermal cycling effects on the flexural strength of glass ceramics fused to titanium. Dent. Mater. J. 2008, 27, 7–15. [CrossRef]
Materials 2020, 13, 4322
31. 32. 33.
38. 39. 40. 41.
42. 43. 44. 45. 46.
15 of 15
Homann, F.; Waddell, J.N.; Swain, M. Influence of water, loading rate and bonder on the adhesion of porcelain to titanium. J. Dent. 2006, 34, 485–490. [CrossRef] Shimoe, S.; Tanoue, N.; Yanagida, H.; Atsuta, M.; Koizumi, H.; Matsumura, H. Comparative strength of metal-ceramic and metal-composite bonds after extended thermocycling. J. Oral Rehabil. 2004, 31, 689–694. [CrossRef] Itinoche, K.M.; Özcan, M.; Bottino, M.A.; Oyafuso, D. Effect of mechanical cycling on the flexural strength of densely sintered ceramics. Dent. Mater. 2006, 22, 1029–1034. [CrossRef] Elekdag-Turk, S.; Turk, T.; Isci, D.; Ozkalayci, N. Thermocycling Effects on Shear Bond Strength of a Self-Etching Primer. Angle Orthod. 2008, 78, 351–356. [CrossRef] Botega, D.M.; Sanchez, J.L.L.; Mesquita, M.F.; Henriques, G.E.P.; Consani, R.L.X. Effects of Thermocycling on the Tensile Bond Strength of Three Permanent Soft Denture Liners. J. Prosthodont. 2008, 17, 550–554. [CrossRef] Ren, X.-W.; Zeng, L.; Wei, Z.-M.; Xin, X.-Z.; Wei, B.; Information, P.E.K.F.C. Effects of multiple firings on metal-ceramic bond strength of Co-Cr alloy fabricated by selective laser melting. J. Prosthet. Dent. 2016, 115, 109–114. [CrossRef] Lenz, J.; Schwarz, S.; Schwickerath, H.; Sperner, F.; Schäfer, A. Bond strength of metal-ceramic systems in three-point flexure bond test. J. Appl. Biomater. 1995, 6, 55–64. [CrossRef] Tuna, S.H.; Pekmez, N.Ö.; Kürkçüoglu, ˘ I. Corrosion resistance assessment of Co-Cr alloy frameworks fabricated by CAD/CAM milling, laser sintering, and casting methods. J. Prosthet. Dent. 2015, 114, 725–734. [CrossRef] Dimitriadis, K.; Papadopoulos, T.; Agathopoulos, S. Effect of Bonding Agent on Metal-Ceramic Bond Strength between Co-Cr Fabricated with Selective Laser Melting and Dental Feldspathic Porcelain. J. Prosthodont. 2019, 28, 1029–1036. [CrossRef] Minesaki, Y.; Murahara, S.; Kajihara, Y.; Takenouchi, Y.; Tanaka, T.; Suzuki, S.; Minami, H. Effect of metal conditioner on bonding of porcelain to cobalt-chromium alloy. J. Adv. Prosthodont. 2016, 8, 1–8. [CrossRef] Lawaf, S.; Nasermostofi, S.; Afradeh, M.; Azizi, A. Comparison of the bond strength of ceramics to Co-Cr alloys made by casting and selective laser melting. J. Adv. Prosthodont. 2017, 9, 52–56. [CrossRef] Xiang, N.; Xin, X.-Z.; Chen, J.; Wei, B. Metal–ceramic bond strength of Co–Cr alloy fabricated by selective laser melting. J. Dent. 2012, 40, 453–457. [CrossRef] Bienia´s, J.; Surowska, B.; Stoch, A.; Matraszek, H.; Walczak, M. The influence of SiO2 and SiO2–TiO2 intermediate coatings on bond strength of titanium and Ti6Al4V alloy to dental porcelain. Dent. Mater. 2009, 25, 1128–1135. [CrossRef] [PubMed] Kononen, M.; Kivilahti, J. Fusing of dental ceramics to titanium. J. Dent. Res. 2001, 80, 848–854. [CrossRef] Könönen, M.; Kivilahti, J. Bonding of low-fusing dental porcelain to commercially pure titanium. J. Biomed. Mater. Res. 1994, 28, 1027–1035. [CrossRef] Itin, V.I. Reaction of Stomatological Porcelain with Titanium and Titanium Nickelide during Sintering. Powder Met. Met. Ceram. 2001, 40, 236–241. [CrossRef] Zinelis, S.; Barmpagadaki, X.; Vergos, V.; Chakmakchi, M.; Eliades, G. Bond strength and interfacial characterization of eight low fusing porcelains to cp Ti. Dent. Mater. 2010, 26, 264–273. [CrossRef] [PubMed] Lu, J.-Y.; Lai, C.-Y.; Almansoori, I.; Chiesa, M.; Almansouri, I. The evolution in graphitic surface wettability with first-principles quantum simulations: The counterintuitive role of water. Phys. Chem. Chem. Phys. 2018, 20, 22636–22644. [CrossRef] [PubMed] Giannozzi, P.; Andreussi, O.; Brumme, T.; Bunau, O.; Nardelli, M.B.; Calandra, M.; Car, R.; Cavazzoni, C.; Ceresoli, D.; Cococcioni, M.; et al. Advanced capabilities for materials modelling with Quantum ESPRESSO. J. Phys. Condens. Matter 2017, 29, 465901. [CrossRef] Nono, M.; Barroso, J.J.; Castro, P. Mechanical behavior and microstructural analysis of alumina–titanium brazed interfaces. Mater. Sci. Eng. A 2006, 435, 602–605. [CrossRef] Ekren, O.; Ozkomur, A.; Ucar, Y. Effect of layered manufacturing techniques, alloy powders, and layer thickness on metal-ceramic bond strength. J. Prosthet. Dent. 2017, 119, 481–487. [CrossRef] © 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).